- Ceramic materials
Ceramic materials are inorganic, non-metallic materials and things made from them. They may be crystalline or partly crystalline. They are formed by the action of heat and subsequent cooling. Clay was one of the earliest materials used to produce ceramics, but many different ceramic materials are now used in domestic, industrial and building products.
- 1 Types of ceramic materials
- 2 Properties of ceramics
- 3 Examples of ceramics materials
- 4 See also
- 5 References
- 6 Further reading
- 7 External links
Types of ceramic materials
A ceramic material may be defined as any inorganic crystalline oxide material. It is solid and inert. Ceramic materials are brittle, hard, strong in compression, weak in shearing and tension. They withstand chemical erosion that occurs in an acidic or caustic environment. In many cases withstanding erosion from the acid and bases applied to it. Ceramics generally can withstand very high temperatures such as temperatures that range from 1,000 °C to 1,600 °C (1,800 °F to 3,000 °F). Exceptions include inorganic materials that do not have oxygen such as silicon carbide. Glass by definition is not a ceramic because it is an amorphous solid (non-crystalline). However, glass involves several steps of the ceramic process and its mechanical properties behave similarly to ceramic materials.
Traditional ceramic raw materials include clay minerals such as kaolinite, more recent materials include aluminium oxide, more commonly known as alumina. The modern ceramic materials, which are classified as advanced ceramics, include silicon carbide and tungsten carbide. Both are valued for their abrasion resistance, and hence find use in applications such as the wear plates of crushing equipment in mining operations. Advanced ceramics are also used in the medicine, electrical and electronics industries.
Crystalline ceramic materials are not amenable to a great range of processing. Methods for dealing with them tend to fall into one of two categories - either make the ceramic in the desired shape, by reaction in situ, or by "forming" powders into the desired shape, and then sintering to form a solid body. Ceramic forming techniques include shaping by hand (sometimes including a rotation process called "throwing"), slip casting, tape casting (used for making very thin ceramic capacitors, etc.), injection moulding, dry pressing, and other variations. (See also Ceramic forming techniques. Details of these processes are described in the two books listed below.) A few methods use a hybrid between the two approaches.
Non-crystalline ceramics, being glasses, tend to be formed from melts. The glass is shaped when either fully molten, by casting, or when in a state of toffee-like viscosity, by methods such as blowing to a mold. If later heat-treatments cause this glass to become partly crystalline, the resulting material is known as a glass-ceramic.
Properties of ceramics
The physical properties of any ceramic substance are a direct result of its crystalline structure and chemical composition. Solid state chemistry reveals the fundamental connection between microstructure and properties such as localized density variations, grain size distribution, type of porosity and second-phase content, which can all be correlated with ceramic properties such as mechanical strength σ by the Hall-Petch equation, hardness, toughness, dielectric constant, and the optical properties exhibited by transparent materials.
Physical properties of chemical compounds which provide evidence of chemical composition include odor, color, volume, density (mass / volume), melting point, boiling point, heat capacity, physical form at room temperature (solid, liquid or gas), hardness, porosity, and index of refraction.
Ceramography is the art and science of preparation, examination and evaluation of ceramic microstructures. Evaluation and characterization of ceramic microstructures is often implemented on similar spatial scales to that used commonly in the emerging field of nanotechnology: from tens of angstroms (A) to tens of micrometers (µm). This is typically somewhere between the minimum wavelength of visible light and the resolution limit of the naked eye.
The microstructure includes most grains, secondary phases, grain boundaries, pores, micro-cracks, structural defects and hardness microindentions. Most bulk mechanical, optical, thermal, electrical and magnetic properties are significantly affected by the observed microstructure. The fabrication method and process conditions are generally indicated by the microstructure. The root cause of many ceramic failures is evident in the cleaved and polished microstructure. Physical properties which constitute the field of materials science and engineering include the following:
Mechanical properties are important in structural and building materials as well as textile fabrics. They include the many properties used to describe the strength of materials such as: elasticity / plasticity, tensile strength, compressive strength, shear strength, fracture toughness & ductility (low in brittle materials), and indentation hardness.
Fracture mechanics is the field of mechanics concerned with the study of the formation and subsequent propagation of microcracks in materials. It uses methods of analytical solid mechanics to calculate the thermodynamic driving force on a crack and the methods of experimental solid mechanics to characterize the material's resistance to fracture and catastrophic failure.
In modern materials science, fracture mechanics is an important tool in improving the mechanical performance of materials and components. It applies the physics of stress and strain, in particular the theories of elasticity and plasticity, to the microscopic crystallographic defects found in real materials in order to predict the macroscopic mechanical failure of bodies. Fractography is widely used with fracture mechanics to understand the causes of failures and also verify the theoretical failure predictions with real life failures.
Thus, since cracks and other microstructural defects can lower the strength of a structure beyond that which might be predicted by the theory of crystalline objects, a different property of the material—above and beyond conventional strength—is needed to describe the fracture resistance of engineering materials. This is the reason for the need for fracture mechanics: the evaluation of the strength of flawed structures.
In this context, Fracture toughness is a property which describes the ability of a material containing a crack to resist fracture, and is one of the most important properties of any material for virtually all design applications. Fracture toughness is a quantitative way of expressing a material's resistance to brittle fracture when a crack is present. If a material has a large value of fracture toughness it will probably undergo ductile fracture. Brittle fracture is very characteristic of materials with a low fracture toughness value. Fracture mechanics, which leads to the concept of fracture toughness, was largely based on the work of A. A. Griffith who, amongst other things, studied the behaviour of cracks in brittle materials.
Ceramic materials are usually ionic or covalent bonded materials, and can be crystalline or amorphous. A material held together by either type of bond will tend to fracture before any plastic deformation takes place, which results in poor toughness in these materials. Additionally, because these materials tend to be porous, the pores and other microscopic imperfections act as stress concentrators, decreasing the toughness further, and reducing the tensile strength. These combine to give catastrophic failures, as opposed to the normally much more gentle failure modes of metals.
These materials do show plastic deformation. However, due to the rigid structure of the crystalline materials, there are very few available slip systems for dislocations to move, and so they deform very slowly. With the non-crystalline (glassy) materials, viscous flow is the dominant source of plastic deformation, and is also very slow. It is therefore neglected in many applications of ceramic materials.
While there are prospects of mass producting blue LEDs from zinc oxide, ceramicists are most interested in the electrical properties that show grain boundary effects.
One of the most widely used of these is the varistor. These are devices that exhibit the property that resistance drops sharply at a certain threshold voltage. Once the voltage across the device reaches the threshold, there is a breakdown of the electrical structure in the vicinity of the grain boundaries, which results in its electrical resistance dropping from several megohms down to a few hundred ohms. The major advantage of these is that they can dissipate a lot of energy, and they self reset – after the voltage across the device drops below the threshold, its resistance returns to being high.
This makes them ideal for surge-protection applications. As there is control over the threshold voltage and energy tolerance, they find use in all sorts of applications. The best demonstration of their ability can be found in electrical substations, where they are employed to protect the infrastructure from lightning strikes. They have rapid response, are low maintenance, and do not appreciably degrade from use, making them virtually ideal devices for this application.
Semiconducting ceramics are also employed as gas sensors. When various gases are passed over a polycrystalline ceramic, its electrical resistance changes. With tuning to the possible gas mixtures, very inexpensive devices can be produced.
Under some conditions, such as extremely low temperature, some ceramics exhibit high temperature superconductivity. The exact reason for this is not known, but there are two major families of superconducting ceramics.
Ferroelectricity and supersets
Piezoelectricity, a link between electrical and mechanical response, is exhibited by a large number of ceramic materials, including the quartz used to measure time in watches and other electronics. Such devices use both properties of piezoelectrics, using electricity to produce a mechanical motion (powering the device) and then using this mechanical motion to produce electricity (generating a signal). The unit of time measured is the natural interval required for electricity to be converted into mechanical energy and back again.
The piezoelectric effect is generally stronger in materials that also exhibit pyroelectricity, and all pyroelectric materials are also piezoelectric. These materials can be used to inter convert between thermal, mechanical, and/or electrical energy; for instance, after synthesis in a furnace, a pyroelectric crystal allowed to cool under no applied stress generally builds up a static charge of thousands of volts. Such materials are used in motion sensors, where the tiny rise in temperature from a warm body entering the room is enough to produce a measurable voltage in the crystal.
In turn, pyroelectricity is seen most strongly in materials which also display the ferroelectric effect, in which a stable electric dipole can be oriented or reversed by applying an electrostatic field. Pyroelectricity is also a necessary consequence of ferroelectricity. This can be used to store information in ferroelectric capacitors, elements of ferroelectric RAM.
The most common such materials are lead zirconate titanate and barium titanate. Aside from the uses mentioned above, their strong piezoelectric response is exploited in the design of high-frequency loudspeakers, transducers for sonar, and actuators for atomic force and scanning tunneling microscopes.
Positive thermal coefficient
Increases in temperature can cause grain boundaries to suddenly become insulating in some semiconducting ceramic materials, mostly mixtures of heavy metal titanates. The critical transition temperature can be adjusted over a wide range by variations in chemistry. In such materials, current will pass through the material until joule heating brings it to the transition temperature, at which point the circuit will be broken and current flow will cease. Such ceramics are used as self-controlled heating elements in, for example, the rear-window defrost circuits of automobiles.
At the transition temperature, the material's dielectric response becomes theoretically infinite. While a lack of temperature control would rule out any practical use of the material near its critical temperature, the dielectric effect remains exceptionally strong even at much higher temperatures. Titanates with critical temperatures far below room temperature have become synonymous with "ceramic" in the context of ceramic capacitors for just this reason.
Optically transparent materials focus on the response of a material to incoming lightwaves of a range of wavelengths. Frequency selective optical filters can be utilized to alter or enhance the brightness and contrast of a digital image. Guided lightwave transmission via frequency selective waveguides involves the emerging field of fiber optics and the ability of certain glassy compositions as a transmission medium for a range of frequencies simultaneously (multi-mode optical fiber) with little or no interference between competing wavelengths or frequencies. This resonant mode of energy and data transmission via electromagnetic (light) wave propagation, though low powered, is virtually lossless. Optical waveguides are used as components in Integrated optical circuits (e.g. light-emitting diodes, LEDs) or as the transmission medium in local and long haul optical communication systems. Also of value to the emerging materials scientist is the sensitivity of materials to radiation in the thermal infrared (IR) portion of the electromagnetic spectrum. This heat-seeking ability is responsible for such diverse optical phenomena as Night-vision and IR luminescence.
Thus, there is an increasing need in the military sector for high-strength, robust materials which have the capability to transmit light (electromagnetic waves) in the visible (0.4 – 0.7 micrometers) and mid-infrared (1 – 5 micrometers) regions of the spectrum. These materials are needed for applications requiring transparent armor, including next-generation high-speed missiles and pods, as well as protection against improvised explosive devices (IED).
In the 1960s, scientists at General Electric (GE) discovered that under the right manufacturing conditions, some ceramics, especially aluminium oxide (alumina), could be made translucent. These translucent materials were transparent enough to be used for containing the electrical plasma generated in high-pressure sodium street lamps. During the past two decades, additional types of transparent ceramics have been developed for applications such as nose cones for heat-seeking missiles, windows for fighter aircraft, and scintillation counters for computed tomography scanners.
In the early 1970s, Thomas Soules pioneered computer modeling of light transmission through translucent ceramic alumina. His model showed that microscopic pores in ceramic, mainly trapped at the junctions of microcrystalline grains, caused light to scatter and prevented true transparency. The volume fraction of these microscopic pores had to be less than 1% for high-quality optical transmission.
This is basically a particle size effect. Opacity results from the incoherent scattering of light at surfaces and interfaces. In addition to pores, most of the interfaces in a typical metal or ceramic object are in the form of grain boundaries which separate tiny regions of crystalline order. When the size of the scattering center (or grain boundary) is reduced below the size of the wavelength of the light being scattered, the scattering no longer occurs to any significant extent.
In the formation of polycrystalline materials (metals and ceramics) the size of the crystalline grains is determined largely by the size of the crystalline particles present in the raw material during formation (or pressing) of the object. Moreover, the size of the grain boundaries scales directly with particle size. Thus a reduction of the original particle size below the wavelength of visible light (~ 0.5 micrometers for shortwave violet) eliminates any light scattering, resulting in a transparent material.
Recently[when?], Japanese scientists have developed techniques to produce ceramic parts that rival the transparency of traditional crystals (grown from a single seed) and exceed the fracture toughness of a single crystal. In particular, scientists at the Japanese firm Konoshima Ltd., a producer of ceramic construction materials and industrial chemicals, have been looking for markets for their transparent ceramics.
Livermore researchers realized that these ceramics might greatly benefit high-powered lasers used in the National Ignition Facility (NIF) Programs Directorate. In particular, a Livermore research team began to acquire advanced transparent ceramics from Konoshima to determine if they could meet the optical requirements needed for Livermore’s Solid-State Heat Capacity Laser (SSHCL). Livermore researchers have also been testing applications of these materials for applications such as advanced drivers for laser-driven fusion power plants.
Examples of ceramics materials
- Barium titanate (often mixed with strontium titanate) displays ferroelectricity, meaning that its mechanical, electrical, and thermal responses are coupled to one another and also history-dependent. It is widely used in electromechanical transducers, ceramic capacitors, and data storage elements. Grain boundary conditions can create PTC effects in heating elements.
- Bismuth strontium calcium copper oxide, a high-temperature superconductor
- Boron nitride is structurally isoelectronic to carbon and takes on similar physical forms: a graphite-like one used as a lubricant, and a diamond-like one used as an abrasive.
- Earthenware used for domestic ware such as plates and mugs.
- Ferrite is used in the magnetic cores of electrical transformers and magnetic core memory.
- Lead zirconate titanate (PZT) was developed at the United States National Bureau of Standards in 1954. PZT is used as an ultrasonic transducer, as its piezoelectric properties greatly exceed those of Rochelle salt.
- Magnesium diboride (MgB2) is an unconventional superconductor.
- Porcelain is used for a wide range of household and industrial products.
- Sialon (Silicon Aluminium Oxynitride) has high strength; high thermal, shock, chemical and wear resistance, and low density. These ceramics are used in non-ferrous molten metal handling, weld pins and the chemical industry.
- Silicon carbide (SiC) is used as a susceptor in microwave furnaces, a commonly used abrasive, and as a refractory material.
- Silicon nitride (Si3N4) is used as an abrasive powder.
- Steatite (magnesium silicates) is used as an electrical insulator.
- Titanium carbide Used in space shuttle re-entry shields and scratchproof watches.
- Uranium oxide (UO2), used as fuel in nuclear reactors.
- Yttrium barium copper oxide (YBa2Cu3O7-x), another high temperature superconductor.
- Zinc oxide (ZnO), which is a semiconductor, and used in the construction of varistors.
- Zirconium dioxide (zirconia), which in pure form undergoes many phase changes between room temperature and practical sintering temperatures, can be chemically "stabilized" in several different forms. Its high oxygen ion conductivity recommends it for use in fuel cells and automotive oxygen sensors. In another variant, metastable structures can impart transformation toughening for mechanical applications; most ceramic knife blades are made of this material.
- Partially stabilised zirconia (PSZ) is much less brittle than other ceramics and is used for metal forming tools, valves and liners, abrasive slurries, kitchen knives and bearings subject to severe abrasion.
- Greskovich, G., et al., Polycrystalline Ceramic Lasers, J. Appl. Phys., Vol. 44, p. 4599 (1973)
- Yoldas, B.E. Monolithic Glass Formation by Chemical Polymerization, J. Mater. Sci., Vol.10, p. 1856 (1975), Deposition and Properties of Optical Oxide Coatings from Polymerized Solutions, Applied Optics, Vol. 21, p. 2960 (1982), An Aqueous Sol–Gel Route to Prepare Transparent Hybrid Materials, J. Mater. Chem., Vol. 17, p. 4430 (2007)
- Ikesue, A., et al., Fabrication and Optical Properties of High Performance Polycrystalline Ceramics of Solid State Lasers, J. Am. Ceram. Soc, Vol. 78, p. 1033 (1995), Polycrystalline Lasers, Optical Materials, Vol. 19, p. 183 (2002)
- Tachiwaki, T., et al., Novel Synthesis of YAG leading to Transparent Ceramics, Solid State Communications, Vol. 119, p. 603 (2001)
- Rabinovitch, Y., et al., Transparent Polycrystalline Neodymium-Doped YAG, Optical Materials, Vol.24, p. 345 (2003)
- Wen, L.,et al., Synthesis of Nanocrystalline Yttria Powder and Fabrication of Transparent YAG Ceramics, J. European Ceramic Soc., Vol. 24, p. 2681, (2004)
- Pradhan, A.K., et al., Synthesis of Neodymium-doped YAG Nanocrystlalline Powders Leading to Transparent Ceramics, Materials Research Bulletin, Vol. 39, p. 1291 (2004)
- Jiang, H., et al., Transparent Electro-Optic Ceramics and Devices, Proc. SPIE, Vol. 5644, p. 380 (2005), www.bostonati.com/whitepapers/SPIE04paper.pdf
- Huie, J.C. and Gentilman, R., Characterization of Transparent Polycrystalline YAG Fabricated from Nanopowders, Window and Dome Technologies and Materials IX, Proc. SPIE, Vol. 5786, p. 251 (2005)
- Barnakov, Yu. A., et al., Simple Route to Nd:YAG Transparent Ceramics, Materials Research Bulletin, Vol. 35, p. 238 (2006)
- Barnakov, Y.A., et al., The Progress Towards Transparent Ceramics Fabrication, Proc. SPIE, Vol. 6552, p. 111 (2007)
- Yamashita, I., et al., Transparent Ceramics, J. Am. Ceram. Soc., Vol. 91, p. 813 (2008)
- M.W. Barsoum, Fundamentals of Ceramics, McGraw-Hill Co., Inc., 1997, ISBN 978-0070055216.
- Green, D.J.; Hannink, R.; Swain, M.V. (1989). Transformation Toughening of Ceramics. Boca Raton: CRC Press. ISBN 0-8493-6594-5.
- W.D. Kingery, H.K. Bowen and D.R. Uhlmann, Introduction to Ceramics, John Wiley & Sons, Inc., 1976, ISBN 0-471-47860-1.
- M.N. Rahaman, Ceramic Processing and Sintering, 2nd Ed., Marcel Dekker Inc., 2003, ISBN 0-8247-0988-8.
- J.S. Reed, Introduction to the Principles of Ceramic Processing, John Wiley & Sons, Inc., 1988, ISBN 0-471-84554-X.
- D.W. Richerson, Modern Ceramic Engineering, 2nd Ed., Marcel Dekker Inc., 1992, ISBN 0-8247-8634-3.
- Onoda, G.Y., Hench, L.L. Eds., Ceramic Processing Before Firing, Wiley & Sons, New York (1979)
- Wachtman, John B. (1996). Mechanical Properties of Ceramics. New York: Wiley-Interscience, John Wiley & Son's. ISBN 0-471-13316-7.
- Advanced Ceramics – The Evolution, Classification, Properties, Production, Firing, Finishing and Design of Advanced Ceramics
- Introduction, Scientific Principles, Properties and Processing of Ceramics
- The American Ceramic Society
- CERAM Research Ltd (formerly The British Ceramic Research Association)
- Worldwide Ceramics Directory
- How pottery is made
- How sanitaryware is made
Wikimedia Foundation. 2010.
Look at other dictionaries:
Ceramic forming techniques — are ways of forming ceramic shapes. This can be used to make everyday tableware from teapots, to engineering ceramics such as computer parts. Methods for forming powders of ceramic raw materials into complex shapes are desirable in many areas of… … Wikipedia
Ceramic petrography — (or ceramic petrology) is a laboratory based scientific archaeological technique that examines the mineralogical and microstructural composition of ceramics and other inorganic materials under the polarising light microscope in order to interpret … Wikipedia
Ceramic water filter — Ceramic water filters are an inexpensive and effective type of water filter, that rely on the small pore size of ceramic material to filter dirt, debris, and bacteria out of water. Contents 1 Method of action 2 Development and expansion 3 See… … Wikipedia
Ceramic armor — is armor used by armored vehicles and in personal armor for its attenuative properties. Contents 1 Design 2 Mechanism 3 Applications 3.1 Personnel … Wikipedia
Ceramic foam — is a tough foam made from ceramics. Manufacturing techniques include impregnating open cell polymer foams internally with ceramic slurry and then firing in a kiln, leaving only ceramic material. The foams may consist of several ceramic materials… … Wikipedia
Ceramic colorants — are added to a glaze or a clay to create color. Carbonates and oxides of certain metals, characterize most colorants including the commonly used cobalt carbonate, cobalt oxide, chrome oxide, red iron oxide, and copper carbonate. These colorants… … Wikipedia
Ceramic engineering — Simulation of the outside of the Space Shuttle as it heats up to over 1,500 °C (2,730 °F) during re entry into the Earth s atmosphere Ceramic engineering is the science and technology of creating objects from inorganic, non metallic… … Wikipedia
Ceramic — A Ming Dynasty porcelain vase dating 1403 1424 … Wikipedia
Ceramic matrix composite — Fracture surface of a fiber reinforced ceramic composed of SiC fibers and SiC matrix. The fiber pull out mechanism shown is the key to CMC properties … Wikipedia
materials science — the study of the characteristics and uses of various materials, as glass, plastics, and metals. [1960 65] * * * Study of the properties of solid materials and how those properties are determined by the material s composition and structure, both… … Universalium